Hot-rolling nanowire transparent electrodes for surface roughness minimization
© Hosseinzadeh Khaligh and Goldthorpe; licensee Springer. 2014
Received: 15 May 2014
Accepted: 2 June 2014
Published: 19 June 2014
Silver nanowire transparent electrodes are a promising alternative to transparent conductive oxides. However, their surface roughness presents a problem for their integration into devices with thin layers such as organic electronic devices. In this paper, hot rollers are used to soften plastic substrates with heat and mechanically press the nanowires into the substrate surface. By doing so, the root-mean-square surface roughness is reduced to 7 nm and the maximum peak-to-valley value is 30 nm, making the electrodes suitable for typical organic devices. This simple process requires no additional materials, which results in a higher transparency, and is compatible with roll-to-roll fabrication processes. In addition, the adhesion of the nanowires to the substrate significantly increases.
KeywordsSilver nanowires Transparent electrode Hot-rolling Surface roughness Adhesion Organic electronics
Transparent electrodes are a required component of many devices such as organic solar cells, electronic displays, and touch screens. The most commonly used transparent conductor is indium tin oxide (ITO). ITO, however, is expensive, not suitable for flexible applications, and requires sputtering, high temperatures, and vacuum for its deposition. Several materials have been proposed to replace ITO such as graphene , carbon nanotubes [2, 3], and copper [4, 5] and silver nanowires [6–8]. Of these, silver nanowire electrodes have been identified as the lead alternative because they have the lowest sheet resistance at a given transparency [9–11]. Not only can silver nanowire electrodes provide the same sheet resistance and transparency as ITO, but they are also highly flexible [12, 13] and inexpensive , and their fabrication is compatible with roll-to-roll processes.
In spite of all the advantages of nanowire electrodes, there are certain issues that need to be addressed before their widespread use in devices. One of these most important issues is their surface roughness. Because there are typically junctions on an electrode where three or more nanowires are stacked on top of one another, maximum peak-to-valley values can reach three times the diameter of the nanowires or more [12, 14]. Nanowires with diameters of 90 nm are commonly used, and so, these electrodes have peak-to-valley values around or exceeding 270 nm. This is problematic for many devices, especially ones that consist of thin layers. In organic electronic devices, for example, the low electron mobility and fast recombination times require organic layers to be less than 100-nm thick (typically 40 to 80 nm depending on the device and materials used) [15, 16]. Several reports where silver nanowire electrodes have been used in organic solar cells have reported lower efficiencies than equivalent devices built on ITO. The rough surface of the nanowire electrodes causes a lower shunt resistance, which increases the dark current and hinders the efficiency of the solar cells [17–19]. The roughness also leads researchers to use a thicker layer of poly(3,4-ethylenedioxythiophene) poly(styrenesulfonate) (PEDOT:PSS) than is typically used on ITO-based devices . This thicker layer decreases transparency and therefore also reduces efficiency. Weak adhesion of nanowires to the substrate is another important issue. Without any special processing, scratches or shear stresses on the surface can easily wipe the nanowires from the surface .
Several papers in the literature have addressed the roughness and adhesion issues of nanowire electrodes. Solutions fall into three general categories. The first involves using a transparent conductive material to fill the spaces between the nanowires [14, 18, 20–22]. Gaynor et al. pressed silver nanowires into a layer of the transparent conductive polymer (PEDOT:PSS) to decrease the root-mean-square (RMS) surface roughness to 12 nm and maximum peak-to-valley values to around 30 nm . Choi et al. instead deposited the PEDOT:PSS layer on top of the nanowire film to achieve an RMS roughness of 52 nm . Chung et al. alternatively used ITO nanoparticles to fill the spaces between the wires and reduced the RMS roughness to 13 nm and the maximum peak-to-valley to below 30 nm. In the latter paper, polyvinyl alcohol (PVA) was also added to the ITO nanoparticle solution to increase the adhesion of the nanoparticle/nanowire film to the substrate . The downside of all these approaches is that to significantly reduce surface roughness, the required thickness of the conductive material needs to be at least three times the diameter of the nanowires. At these thicknesses, there is a reduction in the electrode transparency and consequently the efficiency of the devices due to the limited transparency of the conductive materials .
The second category to reduce roughness is to deposit a transparent but nonconductive polymer on top of the nanowire film [12, 23–25]. This allows a material that is more transparent than PEDOT:PSS or ITO to be used. Using an optical adhesive in this manner, Miller et al. reduced the RMS roughness of silver nanowire films to 8 nm and there was only a 2% change in sheet resistance after an adhesion test . Zeng et al. buried silver nanowires in PVA to reduce the surface RMS to below 5 nm and increase adhesion of the nanowires to the substrate . However, because the polymers used are not conductive, in all these studies the nanowire/polymer composite must be peeled off the original substrate to expose the conductive nanowire-mesh surface, which adds a complex manufacturing step. Although not reported in the literature (to our knowledge), the nanowire film could instead be pressed into a transparent nonconductive polymer, to avoid the peeling step. This technique however would still be less than ideal as an extra polymer layer would still add manufacturing complexity and some devices may not be compatible with the polymer used.
The third category to reduce nanowire electrode roughness is to avoid using an additional polymer and instead press the nanowires into the plastic substrate itself (usually polyethylene terephthalate, PET) [7, 26, 27]. Tokuno et al. mechanically pressed silver nanowire films on PET at room temperature . The resulting RMS surface roughness was 18 nm, which is still quite high. Hauger et al. added to this process by applying heat during pressing to soften the PET substrate . In this latter paper, silver nanowire films on PET were placed facedown on a 165°C stainless steel sheet, and then a rod was rolled over the backside of the substrate. The resulting RMS surface roughness of the rolled electrodes was 27 nm, which is not as smooth as what other methods were able to achieve. After an adhesion test, which was done by applying and then peeling off a piece of scotch tape, the sheet resistance of the electrodes increased more than four times. Furthermore, the high temperature used is not compatible with most plastic substrates, and the maximum peak-to-valley values, which are more important than RMS values in regards to electrical shorts or shunting, were not reported.
This present study uses a roll-to-roll compatible process whereby hot rollers are used to apply heat and mechanical pressure at the same time. The heat results in the softening of the plastic substrate while the mechanical pressure pushes the silver nanowires into the surface of the softened substrate. By embedding the silver nanowires into the substrate surface, the RMS roughness is reduced to 7 nm and the maximum peak-to-valley is 30 nm. A temperature of 80°C was used, which is safe for most plastic substrates. No additional polymers are used which results in higher transparencies, reduces the number of manufacturing steps, and avoids potential incompatibilities between extraneous polymers and some device materials.
Fabrication of electrodes
The sheet resistance of the electrodes was measured by either a four-point probe measurement or a multimeter. The transparencies were recorded with a spectrophotometer, with plain PET as a reference. Atomic force microscopy (AFM) was used to measure surface roughness, and peak-to-valley values were extracted from line scan data collected by Gwiddion software. Tilted scanning electron microscopy (SEM) images were taken of the electrodes, which had been coated with a 10-nm gold layer to prevent electron charging. To determine the level of adhesion, a piece of scotch tape was applied on the silver nanowire film, pressed with a finger, and then peeled off, with the sheet resistance of the electrode being measured before and after. Bending tests were done by bending the electrodes around a rod with a 5-mm radius. The sheet resistance of the electrodes was measured before, after, and during the bending.
Results and discussion
The rollers’ temperature, speed, and spacing were optimized to minimize the surface roughness of the electrode without damaging the silver nanowires and the substrate. A rolling temperature of 80°C was the maximum that the substrate could tolerate before deforming. The rolling speed of 5 mm/s allowed enough time for the substrate to heat up and soften during rolling.
Roughness data of the nanowire electrodes
RMS roughness (nm)
Max peak-to-valley (nm)
Rolled at 80°C
Because different groups use different nanowire diameters for their electrodes, samples were also fabricated from 90-nm-diameter silver nanowires for comparison. The RMS roughness of the annealed 90-nm-diameter nanowire electrodes was 40 nm, and was 10 nm in the hot-rolled samples. The maximum peak-to-valley height values were 150 and 50 nm for the annealed and hot-rolled electrodes, respectively.
Percent change in sheet resistance after the tape test on differently prepared electrodes
Rolled at 80°C
Sheet resistance change after tape test
While bent around a 5-mm rod, the sheet resistance of hot-rolled electrodes increased by less than 1%. When bent 100 times and then returned flat, the resistance was unchanged. In comparison, the sheet resistance of annealed electrodes increased by 3% when bent, and 2% after 100 bending cycles. Thus, the hot-rolled electrodes had slightly better flexibility, perhaps due to the better attachment of the nanowires to the substrate.
This paper demonstrates a hot-rolling process to achieve silver nanowire transparent electrodes with a smooth surface topology and excellent nanowire adhesion to the substrate. An RMS surface roughness of 7 nm was achieved, with a maximum peak-to-valley height of 30 nm. These values meet the smoothness requirements needed for most organic devices. The silver nanowires were successfully embedded in the substrate such that their sheet resistance changed less than 1% after the tape test. This report shows that the surface roughness issue for nanowire electrodes can be easily addressed in a roll-to-roll compatible process without using any additional materials.
atomic force microscopy
indium tin oxide
PSS: poly(3,4-ethylenedioxythiophene) poly(styrenesulfonate)
scanning electron microscope.
This work was supported by the Natural Science and Engineering Research Council (NSERC) of Canada.
- Pang S, Hernandez Y, Feng X, Müllen K: Graphene as transparent electrode material for organic electronics. Adv Mater 2011, 23: 2779–2795. 10.1002/adma.201100304View Article
- Dan B, Irvin GC, Pasquali M: Continuous and scalable fabrication of transparent conducting carbon nanotube films. ACS Nano 2009, 3: 835–843. 10.1021/nn8008307View Article
- Hecht DS, Heintz AM, Lee R, Hu L, Moore B, Cucksey C, Risser S: High conductivity transparent carbon nanotube films deposited from superacid. Nanotechnology 2011, 22: 075201. 10.1088/0957-4484/22/7/075201View Article
- Rathmell AR, Wiley BJ: The synthesis and coating of long, thin copper nanowires to make flexible, transparent conducting films on plastic substrates. Adv Mater 2011, 23: 4798–4803. 10.1002/adma.201102284View Article
- Rathmell AR, Bergin SM, Hua Y-L, Li Z-Y, Wiley BJ: The growth mechanism of copper nanowires and their properties in flexible, transparent conducting films. Adv Mater 2010, 22: 3558–3563. 10.1002/adma.201000775View Article
- Madaria AR, Kumar A, Zhou C: Large scale, highly conductive and patterned transparent films of silver nanowires on arbitrary substrates and their application in touch screens. Nanotechnology 2011, 22: 245201. 10.1088/0957-4484/22/24/245201View Article
- Hu L, Kim HS, Lee J-Y, Peumans P, Cui Y: Scalable coating and properties of transparent, flexible, silver nanowire electrodes. ACS Nano 2010, 4: 2955–2963. 10.1021/nn1005232View Article
- Liu C-H, Yu X: Silver nanowire-based transparent, flexible, and conductive thin film. Nanoscale Res Lett 2011, 6: 75. 10.1186/1556-276X-6-75View Article
- Kumar A, Zhou C: The race to replace tin-doped indium oxide: which material will win? ACS Nano 2010, 4: 11–14. 10.1021/nn901903bView Article
- Hecht DS, Hu L, Irvin G: Emerging transparent electrodes based on thin films of carbon nanotubes, graphene, and metallic nanostructures. Adv Mater 2011, 23: 1482–1513. 10.1002/adma.201003188View Article
- Langley D, Giusti G, Mayousse C, Celle C, Bellet D, Simonato J-P: Flexible transparent conductive materials based on silver nanowire networks: a review. Nanotechnology 2013, 24: 452001. 10.1088/0957-4484/24/45/452001View Article
- Yu Z, Zhang Q, Li L, Chen Q, Niu X, Liu J, Pei Q: Highly flexible silver nanowire electrodes for shape-memory polymer light-emitting diodes. Adv Mater 2011, 23: 664–668. 10.1002/adma.201003398View Article
- De S, Higgins TM, Lyons PE, Doherty EM, Nirmalraj PN, Blau WJ, Boland JJ, Coleman JN: Silver nanowire networks as flexible, transparent, conducting films: extremely high DC to optical conductivity ratios. ACS Nano 2009, 3: 1767–1774. 10.1021/nn900348cView Article
- Choi DY, Kang HW, Sung HJ, Kim SS: Annealing-free, flexible silver nanowire-polymer composite electrodes via a continuous two-step spray-coating method. Nanoscale 2013, 5: 977–983. 10.1039/c2nr32221hView Article
- Pettersson LAA: Enhanced photo conversion efficiency utilizing interference inside organic hetero junction photovoltaic devices. Synth Met 1999, 102: 1107. 10.1016/S0379-6779(98)01389-7View Article
- Li G, Shrotriya V, Yao Y, Yang Y: Investigation of annealing effects and film thickness dependence of polymer solar cells based on poly(3-hexylthiophene). J Appl Phys 2005, 98: 043704. 10.1063/1.2008386View Article
- Lee J-Y, Connor ST, Cui Y, Peumans P: Solution-processed metal nanowire mesh transparent electrodes. Nano Lett 2008, 8: 689–692. 10.1021/nl073296gView Article
- Leem D-S, Edwards A, Faist M, Nelson J, Bradley DDC, de Mello JC: Efficient organic solar cells with solution-processed silver nanowire electrodes. Adv Mater 2011, 23: 4371–4375. 10.1002/adma.201100871View Article
- Krantz J, Richter M, Spallek S, Spiecker E, Brabec CJ: Solution-processed metallic nanowire electrodes as indium tin oxide replacement for thin-film solar cells. Adv Funct Mater 2011, 21: 4784–4787. 10.1002/adfm.201100457View Article
- Noh Y-J, Kim S-S, Kim T-W, Na S-I: Cost-effective ITO-free organic solar cells with silver nanowire–PEDOT:PSS composite electrodes via a one-step spray deposition method. Sol Energy Mater Sol Cells 2014, 120(Part A):226–230.View Article
- Gaynor W, Burkhard GF, McGehee MD, Peumans P: Smooth nanowire/polymer composite transparent electrodes. Adv Mater 2011, 23: 2905–2910. 10.1002/adma.201100566View Article
- Chung C-H, Song T-B, Bob B, Zhu R, Yang Y: Solution-processed flexible transparent conductors composed of silver nanowire networks embedded in indium tin oxide nanoparticle matrices. Nano Res 2012, 5: 805–814. 10.1007/s12274-012-0264-8View Article
- Yu Z, Li L, Zhang Q, Hu W, Pei Q: Silver nanowire-polymer composite electrodes for efficient polymer solar cells. Adv Mater 2011, 23: 4453–4457. 10.1002/adma.201101992View Article
- Zeng X-Y, Zhang Q-K, Yu R-M, Lu C-Z: A new transparent conductor: silver nanowire film buried at the surface of a transparent polymer. Adv Mater 2010, 22: 4484–4488. 10.1002/adma.201001811View Article
- Miller MS, O’Kane JC, Niec A, Carmichael RS, Carmichael TB: Silver nanowire/optical adhesive coatings as transparent electrodes for flexible electronics. ACS Appl Mater Interfaces 2013, 5: 10165–10172. 10.1021/am402847yView Article
- Tokuno T, Nogi M, Karakawa M, Jiu J, Nge TT, Aso Y, Suganuma K: Fabrication of silver nanowire transparent electrodes at room temperature. Nano Res 2011, 4: 1215–1222. 10.1007/s12274-011-0172-3View Article
- Hauger TC, Al-Rafia SMI, Buriak JM: Rolling silver nanowire electrodes: simultaneously addressing adhesion, roughness, and conductivity. ACS Appl Mater Interfaces 2013, 5: 12663–12671. 10.1021/am403986fView Article
- Ellmer K: Past achievements and future challenges in the development of optically transparent electrodes. Nat Photonics 2012, 6: 809–817. 10.1038/nphoton.2012.282View Article
- Al-Dahoudi N, Aegerter MA: Wet coating deposition of ITO coatings on plastic substrates. J Sol-Gel Sci Technol 2003, 26: 693–697. 10.1023/A:1020777500940View Article
- Weaver MS, Michalski LA, Rajan K, Rothman MA, Silvernail JA, Brown JJ, Burrows PE, Graff GL, Gross ME, Martin PM, Hall M, Mast E, Bonham C, Bennett W, Zumhoff M: Organic light-emitting devices with extended operating lifetimes on plastic substrates. Appl Phys Lett 2002, 81: 2929–2931. 10.1063/1.1514831View Article
- Hong Y, He Z, Lennhoff NS, Banach DA, Kanicki J: Transparent flexible plastic substrates for organic light-emitting devices. J Electron Mater 2004, 33: 312–320. 10.1007/s11664-004-0137-3View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.